HAL Id: hal-01680977
https://hal.archives-ouvertes.fr/hal-01680977Submitted on 11 Jan 2018
HAL is a multi-disciplinary open access archive for the deposit and dissemination of sci-entific research documents, whether they are pub-lished or not. The documents may come from teaching and research institutions in France or abroad, or from public or private research centers.
L’archive ouverte pluridisciplinaire HAL, est destinée au dépôt et à la diffusion de documents scientifiques de niveau recherche, publiés ou non, émanant des établissements d’enseignement et de recherche français ou étrangers, des laboratoires publics ou privés.
Morphology and surface reactivity relationship in the
Li1+xMn2–xO4 spinel with x = 0.05 and 0.10: a
combined first-principle and experimental study
Ambroise Quesne-Turin, Germain Vallverdu, Delphine Flahaut, Joachim
Allouche, Laurence Croguennec, Michel Ménétrier, Isabelle Baraille
To cite this version:
Ambroise Quesne-Turin, Germain Vallverdu, Delphine Flahaut, Joachim Allouche, Laurence Croguen-nec, et al.. Morphology and surface reactivity relationship in the Li1+xMn2–xO4 spinel with x = 0.05 and 0.10: a combined first-principle and experimental study. ACS Applied Materials & Inter-faces, Washington, D.C. : American Chemical Society, 2017, 9 (51), pp.44922-44930. �10.1021/ac-sami.7b15249�. �hal-01680977�
Morphology and surface reactivity relationship in
spinel with x = 0.05 and 0.10:
A combined first-principle and experimental study
Ambroise Quesne-Turin1,2,3 , Germain Vallverdu1,3* , Delphine Flahaut1,3 , Joachim Allouche1 , Laurence Croguennec2,3 , Michel Ménétrier2,3
and Isabelle Baraille1,3
CNRS/ Univ Pau & Pays Adour, Institut des Sciences Analytiques et de Physico-chimie pour
l’Environnement et les Matériaux, UMR5254, 64000, Pau, France
CNRS, Univ. Bordeaux, Bordeaux INP, ICMCB UPR 9048, F-33600 Pessac, France
RS2E, Réseau Français sur le Stockage Electrochimique de l’Energie, FR CNRS 3459,
F-80039 Amiens Cedex 1, France
Surface reactivity, XPS, spinel positive electrode materials, stoichiometry, first-principle
This paper focuses on the surface reactivity of two spinel samples with different
stoichiometries and crystal morphologies, namely Li1+xMn2-xO4 with x = 0.05 and x =0.10.
LiMn2O4 compounds are good candidates as positive electrode of high power lithium-ion
batteries for portable devices. The samples were investigated using both experimental and
theoretical approaches. On the experimental point of view there were characterized in depth from
XRD, SEM and XPS analyses. Then the reactivity was investigated through the adsorption of
(SO2) gaseous probes, in controlled conditions, followed by XPS characterization. First-principle
calculations were conducted simultaneously in order to investigate the electronic properties and
the reactivity of relevant surfaces of an ideal LiMn2O4 material. The results allow us to conclude
that the reactivity of the samples is dominated by an acido-basic reactivity and the formation of
sulfite species. Nonetheless, on the x = 0.05 sample, both sulfite and sulfate species are obtained,
the later, in lesser extent, corresponding to a redox reactivity. Combining, experimental and
theoretical results, this redox reactivity could be associated to the presence of a larger quantity of
The LiMn2O4 spinel material is a good candidate at the positive electrode of high power
lithium-ion batteries for portable devices. Its theoretical capacity is approximately 140 mAh.g-1
as much as LiCoO2, still the most commonly used positive electrode of commercialized
. Contrary to LiCoO2, LiMn2O4 is considered as a non-toxic and low cost material
with an operating voltage of 4.1 V vs. Li+
/Li. The key issue for LiMn2O4 is a fast capacity fading
upon cycling or storage at a temperature higher than 50°C, which is especially in relationship
with the transition metal dissolution into the electrolyte3,4. It is this latter key issue that we want
to address by considering the specific reactivity of different surfaces of the spinel structure. As
the electrolyte contains different alkyl carbonates as solvents and a Li salt (for instance LiPF6),
different reactions can occur with LiMn2O4. Dissolution of manganese in the electrolyte
(solid) → Mn 4+
(solid) + Mn 2+
(solution)) has been significantly observed for LiMn2O4 5,6
. In order to
circumvent this issue, the use of an alternative electrolyte, such as LiB(C2O4)2 4
, or manganese
and oxygen atoms substitutions by aluminum and fluorine atoms3
, respectively, was considered
and lead to an improvement of cycling properties at high temperature. Even if more limited, the
LiMO2 layered oxides (M = Mn, Ni, Co) suffer also from transition metal dissolution. To
improve their electrochemical performance at high potential, the formation of a coating with
Al2O3 for example has been revealed as a fruitful method to modify the surface reactivity of the
material toward the electrolyte. Previously, we studied on the basis of XPS analysis and
first-principal calculations, the surface reactivity of LiCoO2 and NMC materials and the effect of a
Al2O3 coating 7–9
versus gaseous probes. We evidenced that the amount of adsorbed species and
their adsorption mode (redox and/or acid/base) are governed by the nature of the transition metal
decreasing the active site concentration and modifying the adsorption mode of the gaseous probe.
For LiCoO2, the coating modifies the surface reactivity with the identification of both sulfate and
sulfite species, which is in line with a change in the adsorption mode from redox toward
acid−base after Al/Co substitution10
. In the case of NMC materials, the phenomenon is more
complex related to the cation mixing effect.
In this paper, we studied the surface reactivity of Li1+xMn2-xO4 (x = 0.05 and 010) spinel
materials showing different stoichiometry and morphology. We performed the adsorption of a
gaseous probe (SO2) on the materials, in controlled conditions and used both XPS analyses and
first-principle calculations to identify the adsorption mode of SO2 on the surface and characterize
its reactivity. We also determined the nature of the active sites on the material surface and
quantify their concentration.
2. MATERIALS AND METHODS
2.1. The two samples Li1+xMn2-xO4 (x = 0.05, 0.10)
Two samples of Li1+xMn2-xO4 were prepared for x = 0.05 and 0.10 according to the method
described in details by Masquelier et. al.11
, i.e. by mixing Li2CO3 and MnO(OH) in
stoichiometric amounts according to the target composition and by heating the obtained mixture
at 400 °C for 2 h and at 800 °C for 20 h in air. An intermediate grinding was performed and the
powder was cooled down at 10 °C/min. As described in details in reference 12 the two spinel
materials crystallize in the cubic 𝐹𝑑3𝑚 space group, the manganese ions occupying the 16d
octahedral sites of a cubic closed-packed oxygen (32e sites) array. The MnO6 octahedra are
containing channels where the lithium ions occupy 8a tetrahedral sites. In the case of Li1+xMn
2-xO4, a partial substitution of lithium for manganese is observed in the 16d sites. The two samples
were characterized in depth combining chemical analyses by inductively coupled plasma optical
emission spectrometry, and structural analyses by X-ray and neutron diffraction as reported in
reference 13. The more overlithiated the spinel phase Li1+xMn2-xO4, the smaller is the lattice
parameter (8.2484(2) Å for LiMn2O4, 8.2307(4) Å for Li1.05Mn1.95O4 and 8.2188(3) Å for
Li1.10Mn1.90O4), in good agreement with a higher average oxidation state for manganese (ionic
radii of 0.58 Å for Mn3+
versus 0.53 Å for Mn4+
as required for charge compensation of the
lithium excess within the host structure. Indeed, 3Mn3+
ions are replaced in the 16d sites by (1Li+
), with a general formula Li1+xMn 4+
1-3xO4. 44% and 37% of the manganese ions
are thus expected to be Mn3+
in Li1.05Mn1.95O4 and Li1.10Mn1.90O4 respectively. Note that the
specific areas of the two materials have been determined by a Micromeritic ASAP 2010, using
the Brunauer–Emmett–Teller (BET) theory15
and were found to be very similar, below 2 m2
2.2.Scanning Electron Microscopy (SEM)
The surface morphology of the samples was analyzed using a JEOL JAMP 9500F Auger
Nanoprobe microscope under Ultra High Vacuum conditions (< 2 x10-9
mbar) fitted with a
Schottky field emission electron gun, using a conventional secondary electron detector (SED) in
the analysis chamber. The analyses were performed using a beam voltage of 30 keV and a beam
current of 2 nA. The materials were gold-sputtered with a Denton Vacuum Desk V metalizer
before being mounted on the sample holder.
The SO2 adsorption was performed in a Micromeritic Autochem 2920 Analyzer. A first step
dedicated to the cleaning of the powders surface was conducted in order to desorb all the
physisorbed species. The Li1+xMn2-xO4 powders were introduced in the silica reactor, and then
submitted to an argon flow at 350 °C for 4 h.
The powders were then maintained at 80 °C for 1 h under a Helium flow to ensure that the next
step, gas probe adsorption, was performed on a stable surface. Finally, the adsorption of SO2 at
the surface of Li1+xMn2-xO4 was performed at 350 °C for 15 min under a gas flow (50 mL·min −1
containing 0.02% of SO2 in helium. Samples were kept under a He flow at 80 °C to remove the
physisorbed species from the samples surface. The gas probe adsorption has been performed
three times for most samples to ensure the reproducibility of the experiment. After adsorption,
the samples were transferred into a glove box before being analyzed, without being submitted to
The choice of the SO2 gaseous probe was based on the small molecule size and its acidic
strength. The identification of adsorbed species as well as the involved mechanisms can be easily
obtained by X-ray photoelectron spectroscopy by considering the large binding energy (B.E.)
scale (almost 10 eV16,17
) of the S 2p core peaks depending of the chemical environments. The
SO2 gaseous probe can be adsorbed on the surface, either according to basic/acidic and/or to
. If the adsorption is driven by an acid/base mode, SO3
sulfite species will
be formed at the surface characterized by a B.E. of the S 2p3/2 core peak at ~167.5 eV. In case of
redox adsorption mode, the adsorption will lead to the formation of SO4
characterized by a B.E. of the S 2p3/2 core peak at ~169.0 eV 18
Quantitative information can also be obtained with the evaluation of the S/Mn atomic ratios,
deduced from XPS analysis of the core peaks of the adsorbed molecules (S 2p for SO2 gas probe)
as well as the metals (Mn 2p for Mn) in the electrode material.
2.4. X-Ray Photoelectron Spectroscopy (XPS)
The XPS analyses were performed on a Kratos Axis Ultra spectrometer with a focused
monochromatized Al Kα radiation. The applied current and voltage were of 12 mA and 12 kV
respectively. The spot size was of 700x400 µm2
. The powders were placed on a Cu double tape
fixed on the sample holder. The samples preparation, for XPS measurements, was performed in a
glove box and transferred to the one which is directly connected to the XPS spectrometer. The
pressure in the analysis chamber was ca. 5 x 10-9
mbar. The spectra were calibrated in B.E. scale
from the Mn 2p3/2 peak of Mn 4+
at 642.3 eV.
2.5. Theoretical calculation
Periodic Density Functional Theory (DFT) calculations were performed to estimate the relative
stability of crystalline surfaces of the materials, to compute the adsorption energies of the
gaseous probes and to investigate the underlying electronic processes. All calculations were
performed with the Vienna Ab initio Simulation Package19,20
(VASP). The wave-functions were
described in the Projector Augmented Wave21
(PAW) formalism using a plane waves basis set
and a cut-off energy of 550 eV. All calculations were done using the GGA exchange and
correlation functional of Perdew and Wang22,23
(PW91). The Brillouin zone integration was done
using a 4×4×4 or 4×4×1 k-points mesh uniformly distributed around the Γ point of the reciprocal
localized on the manganese atoms and requires to perform calculations using the DFT+U
formalism. We used the implementation of the rotationally invariant approximation of Dudarev
, where U and J are melted in a single Ueff = U - J parameter, and we adopted the value
Ueff = 4.84 eV from the work of Xu et al 1
. All calculations were carried out considering spin
polarization with ferromagnetic ordering. Charge calculations were performed by using Bader’s
. For bulk calculations, all degrees of freedom were fully relaxed whereas
the cell shape and volume were kept fixed and only atomic positions of the first atomic layers
were relaxed in the case of surface calculations.
We performed calculation on bulk and surface models of LiMn2O4 and analyzed the atomic
charges and the magnetic moments, in particular, to determine the oxidation state of the
manganese atoms. Calculations were performed in similar conditions for MnII
O2 as references to determine standard values for theMn magnetic moments. They lead to
4.7, 4.0 and 3.4 µB for Mn 2+
respectively. The details of these calculations are
provided in Supporting Information, Table 1.
Figure 1. SEM images of Li1+xMn2-xO4. (a) and (b) for x = 0.05, (c) and (d) for x = 0.10. Insets
in the b and d images give schematic representation of the central particles. The crystallographic
faces are given with different colors depending on their orientation: green for (111), blue for
The morphology of the materials was characterized by scanning electron microscopy. As
displayed in the crystal sizes are in a range of 200-1000 nm. The Li1.05Mn1.95O4 material,
presented in Figure 1 a-b, exhibits truncated surfaces at the edges and vertexes of the octahedral
crystals. On the basis of a previous work of Kim et al27
, the surface orientations can be assumed
to correspond to the lattice planes (111), (001) and (110) which are commonly observed in the
case of cubic lattices (see the graphical inset given in Figure 1 b). The crystal morphology
appears similar for the Li1.10Mn1.90O4 material. Nonetheless, on the crystal displayed on Figure 1
d, the (110) lattice plane appears in a lesser extent.
XPS analyses have been performed on bare and adsorbed materials. The Mn 2p, Mn 3s, O 1s,
Li 1s, S 2p and C 1s core peaks have been recorded to follow the evolution of the electronic
structure of the materials after SO2 adsorption and to identify the nature and the concentration
of the adsorbed species.
Figure 2. Mn 2p (a) and O 1s (b) core peaks for Li1+xMn2-xO4 materials with x = 0.05 and x =
0.10, before and after SO2 adsorption. Blue and red curves correspond to the contributions of
x = 0.05 x = 0.10 B.E. (eV) At. % B.E. (eV) At. % Mn 2p3/2 642.3 17.5 642.3 13.9 O 1s 529.9 26.7 529.9 22.1 531.5 11.6 531.7 9.9 38.3 32.0 C 1s 285.0 22.4 285.0 37.1 286.5 6.3 286.4 5.4 287.8 2.6 287.8 0.8 288.9 1.6 289.0 3.2 32.9 46.5 Li 1s 54.2 11.3 54.2 7.6
Table 1. Binding energies and atomic percentages determined from XPS analysis for Li1+xMn
2-xO4 materials with x = 0.05 and 0.1.
The XPS Mn 2p spectra of the spinel materials are given before and after adsorption in Figure
2 a. They consist in the two main components Mn 2p3/2 and Mn 2p1/2, due to the spin orbit
coupling, and satellites associated to those main peaks located at 11 eV toward the higher
binding energy side. The satellite associated to the Mn 2p3/2 component is hidden by the Mn 2p1/2
component. The area ratio between the Mn 2p3/2 / Mn 2p1/2 is 2:1. The overall envelope of
Mn 2p3/2 peak evidences two oxidation states for the manganese cations according to the shoulder
observed for the at 641.4 eV. The Mn 2p spectra can be decomposed in two contributions due to
(641.4 eV) and Mn4+
(642.3 eV) cations. This identification of the mixed valency of the
manganese cation at the surface is confirmed by the Mn 3s spectra (Figure S2). Actually, the
therefore to a splitting of the Mn 3s peak in two components for which the B.E. splitting value is
directly related to the Mn oxidation state. The B.E. splitting values for the Li1+xMn2-xO4 is 4.9 eV
for x = 0.05 and 4.8 eV for x = 0.10. Those values intermediate between those reported for a pure
(4.5 eV and 5.5 eV28
respectively) confirm the mixed valence state (Mn3+/4+
reported in the literature29
The ratio of Mn3+
can be determined from the Mn 2p spectra of spinel materials. For
this purpose, a decomposition of the Mn 2p peaks has been performed in an accurate manner
described in Figure S1. We obtained roughly the same results for the two materials, 56 ± 1% and
54 ± 2% of Mn3+
species in the Li1.05Mn1.95O4 and the Li1.10Mn1.90O4 materials, respectively. It
reveals - by comparison with the expected average content in Mn3+
within Li1+xMn2-xO4 (44% for
x = 0.05 and 37% for x = 0.10) - that manganese ions are partially reduced at the surface of the
The O 1s spectra of the bare materials, given in Figure 2b, present two contributions, one
at 529.7 eV associated to the oxygen anions of the materials, and a second one at 531.5 eV
related to the under-coordinated oxygen anions from the surface10. The O 1s signal around
533 eV corresponds to the oxygenated adsorbed species. In the same way, the Li 1s core peaks
(Figure S3) located at 54.3 eV is associated to the lithium in the spinel structure.
The atomic percentages are gathered in Table 1. The stoichiometry of the spinel surface
determined from XPS core peaks are Li1.25Mn1.95O2.97 and Li1.04Mn1.90O3.2 respectively for x = 0.05
and x = 0.10. The oxygen content is underestimated as the determination of the stoichiometry is
based only on the contribution of oxide anion (529.7 eV). Thus, oxygen atoms coordinated to Mn
531.5 eV. It may be noted a slight deviation of the Li content from the nominal stoichiometry at
the surface. The Li/Mn ratio is substantially for the x = 0.05 material larger than expected from
nominal values (0.64 and 0.55 against 0.54 and 0.58 for, respectively, x = 0.05 and 0.1).
Nonetheless, the XPS results are consistent with the manganese valence values expected from
XRD results, corresponding to a slight increase of the Mn4+
concentration (44% in the
Li1.05Mn1.95O4 and 46% in the Li1.10Mn1.90O4 vs. 56% and 63%). The discrepancy between the XPS
and nominal stoichiometry is associated to the depth of the XPS analysis (5 nm at most) and thus
reflects usual surface effects.
3.2.2. After SO2 adsorption
For the adsorbed materials, the atomic percentages obtained from XPS analyses are gathered in
x = 0.05 x = 0.10 B.E. (eV) At. % B.E. (eV) At. %
Mn 2p3/2 642.3 18.7 642.3 13.5 O 1s 529.9 30.9 529.8 23.3 531.5 13.2 531.6 19.6 44.1 42.8 C 1s 284.8 20.9 284.1 24.9 286.3 2.6 285.7 4.3 288.0 0.2 287.6 0.4 288.6 0.6 288.1 2.3 24.3 31.9 S 2p3/2 168.5 0.9 168.4 2.2 169.3 0.4 1.3 2.2 Li 1s 54.2 11.6 54.0 9.5
Table 2. Binding energies and atomic percentages determined from XPS analysis for the
Li1+xMn2-xO4 materials after SO2 adsorption.
The stoichiometry of the surface (considering the Li/Mn ratio) is not impacted by the
adsorption for the nominal composition x= 0.05 as we have found a material stoichiometry of
Li1.21Mn1.95O3.22. For x= 0.01, the stoichiometry of Li1.33Mn1.90O3 corresponds to an increase of the
Li/Mn ratio (0.7 after adsorption instead of 0.55 before).
First, we consider the S 2p spectra associated to the sulfur issued from the SO2 gas probe,
Figure 3. Due to the spin orbit coupling, the S 2p core peaks consist of two main components, S
the adsorbed species are different for the two spinel materials. The S 2p spectrum of
Li1.10Mn1.90O4 can be decomposed into one doublet for which the S 2p3/2 B.E. value is 168.4 eV.
In the case of the Li1.05Mn1.95O4 material, two doublets are needed to fit the experimental
spectrum, with an S 2p3/2 B.E. of 168.5 and 169.3 eV. Based on previous studies 7,10,18
expected B.E. values of the S 2p3/2 components after SO2 adsorption are 167 eV and 169 eV,
respectively, in the case of the formation of sulfite and sulfate species at the materials surface. In
this study, the B.E.s of the S 2p3/2 components are slightly larger. Moreover, Flahaut et al. 17
reported an S 2p3/2 B.E. of 167.9 eV and 169.6 eV for the dipropylsulfate and dimethylsulfite,
respectively. Thus, we can suggest that the SO2 gas probe is adsorbed as sulfite at the
Li1.10Mn1.90O4 surface, and both as sulfate and sulfite species for Li1.05Mn1.95O4. The adsorption
mechanisms are thus different: a unique acid/base adsorption mode on the Li1.10Mn1.90O4 surface
and both acid/base (69%) and redox (31%) modes on the Li1.05Mn1.95O4 surface. Moreover, the
concentration of adsorbed species obtained from XPS analyses through the S/Mn ratio, leads to
significantly different values, namely 0.1 and 0.2 for Li1.05Mn1.95O4 and Li1.10Mn1.90O4
Figure 3. S 2p core peaks after SO2 adsorption on Li1+xMn2-xO4 materials with x = 0.10 (top
panel) and x = 0.05 (bottom panel).
The O 1s spectra exhibits a significant rise of the component located at 531.5 eV (Figure 2b.)
upon adsorption. Moreover, the area ratio between the oxygen components associated to
adsorbed species and to oxygen anions of the material is higher for x = 0.10 which is consistent
with the difference in the adsorbed species concentrations obtained from the S/Mn ratios (S/Mn
ratio = 0.1 and 0.2 for Li1.05Mn1.95O4 and Li1.10Mn1.90O4, respectively).
In contrast, no significant difference (considering the whole envelope shape, components B.E.,
spectra after SO2 adsorption for the two Li1+xMn2-xO4 materials. Looking at the spectra more
closely, we can detect tiny variations of the manganese spectra after adsorption for the
Li1.05Mn1.95O4. First, the determination of the manganese valence from the Mn 2p core peaks
highlights an interesting evolution of the manganese electronic structure versus SO2 adsorption
for this composition. The manganese valence has decreased only slightly; 60 ± 1% of the Mn 2p
signal is assigned to Mn3+
after adsorption instead of 56 ± 1% before adsorption. This result
reveals that the redox adsorption mode induces an electronic transfer between the SO2 gas probe
and the Mn4+
present at the surface for the x = 0.05 material. In contrast, this effect does not
appear in the XPS spectra for the x=0.10 material.
3.3. Computational results
In order to analyze more deeply the electronic processes associated to the surface reactivity, a
computational study of the bare surfaces of LiMn2O4 was undertaken, followed by SO2
adsorption on various surfaces of LiMn2O4. Computational accuracy was first checked on the
bulk properties of an ideal LiMn2O4 crystal, depicted in Figure 4a. The calculated value of the
lattice parameter is a = 8.427 Å in good agreement with the experimental one30 of 8.251 Å with a
relative deviation of 2%. The magnetic moment calculated on manganese for a ferromagnetic
arrangement is 3.8 µB, corresponding to a Mn 3+
mixed valence state for manganese in good
agreement with the mixed valence state observed from XPS measurement, and with the 50%
Figure 4. (a) bulk structure of an ideal LiMn2O4 structure. LiO4 tetrahedra are in green and
MnO6 octahedra in purple, (b) particles shape representation; (c-f) side views of the first atomic
layers of the surface models used in the calculations: (c) (111) surface, (d) (001) surface, (e)
(110) surface and (f) (113) surface. Li, Mn and O atoms are in green, purple and red respectively.
In figures (e) and (f), the numbers are labelleds used in the main text.
3.3.1. Bare surfaces
We considered the surfaces observed in the truncated octahedron (Figures 1b and 1d) which
are assumed to be (111), (001), (110) and (113) as suggested by Kim et al.25
. Following the work
of Warburton et al.31
thermodynamics conditions, we selected the more relevant slab models for each surface on the
basis of the thermodynamic stability in a broad range of electrochemical conditions. The selected
models are depicted in Figure 4c-4f. Warburton et al.31
showed that the surface formation
energies of the (110) and (113) surfaces are higher than those of the (111) and (001) surfaces.
These results are consistent with the shape of the particles we obtained (Figures 1b and 1d)
where the (111) and (001) surfaces exhibit the largest area.
The (111) surface model, called Li-rich model by Warburton et al.31
(Figure 4c) is terminated
by a lithium layer which enhances the surface stability. This lithium layer is stacked on top of a
sheet of MnO6 octahedra. The computed magnetic moments of the manganese atoms in the
sub-surface layer are 3.3 µB for 2/3 of the manganese atoms, and 3.9 µB for 1/3 of the manganese
atoms, corresponding to Mn4+
species respectively, according to the calculations on the
reference compounds (see Supporting Information, Table S1).
The (001) surface model, called Mn/O (001) by Warburton et al.31
(Figure 4d) is the most
stable among the (001) surface composition on a broad range of thermochemical conditions
(oxidizing conditions and electrode potential versus Li+/Li potential). It consists in a stacking of
Mn2O4 and Li layers, the termination layers being an Mn2O4 sheet with manganese atoms in an
ML5 environment. The computed magnetic moments of manganese atoms on the surface layer
are 4.0 µB, and correspond to Mn 3+
species. From the top to the core of the slab model, the
computed magnetic moments are 3.4 µB, 3.6 µB and 3.8 µB which is the bulk value,
corresponding to an increasing content in Mn3+
The (110) surface model, called Li/O (110) by Warburton et al.31
(Figure 4e) follows a
layer. This oxygen layer completes the manganese octahedra at the surface, leading to an
enhanced stability. The magnetic moments of the sub-surface manganese atoms are 3.3 µB,
corresponding to Mn4+
. As already observed for the (001) surface model, from the top to the core
of the slab model, the computed magnetic moments increase corresponding to an increasing
proportion of Mn3+
species. The oxygen atoms of the last atomic layer, label 1 in Figure 4e,
exhibit a lower electronic charge of -0.76 e instead of -1.07 e in the bulk of LiMn2O4. This is
attributed to the low coordination of these oxygen atoms which present only two cation
neighbors instead of four in the bulk structure.
The (113) surface model, called Li/Mn/O by Warburton et al.31
(Figure 4f) is considered as a
high-index surface and can be described as a stacking of Mn2O4 and Li layers, as the (001)
surface, but twisted around an in-plane axis by about 45°. At the surface layer, this leads to
manganese atoms in an ML5 environment which exhibit magnetic moments of 4.0 µB for 2/3 of
the manganese atoms (label 1, Figure 4f), and 2.8 µB for 1/3 of the manganese atoms (label 2,
Figure 4f), corresponding to Mn3+
The four models described above present various oxidation states for the manganese atoms on
the last surface layers and therefore suggest different behaviors upon adsorption of a gas probe.
The variety of the considered models will allow us to establish the relationship between the
chemical composition and the surface reactivity.
3.3.2. Surfaces after SO2 adsorption
Calculations of the adsorption of an SO2 probe molecule were performed on the four surface
models described above. Sulfite and sulfate sites were probed in an exhaustive way by
geometries were obtained by placing the SO2 molecule either in a tetrahedral (bridge sites) or a
trigonal (top sites) environment for the sulfur atom leading to the formation of sulfate or sulfite
species, respectively. For the sulfite adsorption, the sulfur atom is located 1.55 Å away from the
oxygen atom belonging to the surface. For the sulfate adsorption, the sulfur atom is located
initially 1.55 Å away from the barycenter of two surface oxygen atoms. The geometry is then
fully relaxed and the adsorption energy, 𝐸&'(, is computed from
𝐸&'( = 𝐸(*+,&-./012− (𝐸(*+,&-. + 𝐸012)
where 𝐸(*+,&-./012 is the energy of the adsorbed system, 𝐸(*+,&-. is the bare surface energy
and 𝐸012 the energy of an isolated SO2 molecule obtained from the calculation of an isolated SO2
molecule in a cubic box of 10 Å length. The adsorption energies and the electronic transfers,
from the SO2 molecule towards the surface, of the most stable sulfite and sulfate adsorptions are
gathered in Table 3. The electronic transfers were computed from the Bader charges analysis.
Surface species Eads (eV) ΔqSO2
(111) Sulfite -1.12 -0.4 (001) Sulfite -1.49 -0.1 (110) Sulfite -0.89 -0.2 (110) Sulfate -2.71 1.1 (113) Sulfite -1.14 -0.4 (113) Sulfate -4.29 1.0
Table 3. Adsorption energy (Eads) and electronic transfer, Δq, from SO2 towards the surface for
Whatever the surface, the electronic transfer is about one electron from the SO2 molecule
toward the surface in the case of the formation of sulfate species, while a smaller transfer, of at
most 0.4 electron from the surface toward the SO2 molecule, is obtained in the case of sulfite
species. This agrees with the redox reactivity associated with the sulfate formation and the
acid-base reactivity associated with the formation of sulfite species8,9
. The range of computed
adsorption energies indicates the formation of chemisorbed species, stable enough to be observed
by XPS characterizations under ultra-high vacuum conditions.
Figure 5. SO2 adsorption on LiMn2O4 surfaces after structural relaxation. (a) and (b) Sulfite
adsorption mode on (111) and (001) surfaces respectively, (c) and (d) sulfate adsorption mode on
In the case of the (111) and (001) surfaces, the formation of sulfite species is favored with an
adsorption energy of -1.12 and -1.49 eV respectively. The formation of sulfate species was also
considered but actually leads to the formation of sulfite species. The relaxed geometries of the
most stable adsorptions are depicted in Figure 5a and Figure 5b for surfaces (111) and (001)
respectively. In both cases, the adsorbed molecule is stabilized by the formation of secondary
interactions between oxygen atoms of SO2 and cations of the last atomic layer of the surface. In
the case of the (001) surface, the oxygen atoms of SO2 complete the coordination sphere of the
manganese atoms in order to place them in an ML6 environment corresponding to the bulk
structure. The lengths of these bonds are similar to other Mn-O bonds in the bulk octahedra
(2.03/2.14 Å vs 1.96 Å). For both surfaces, the electronic structure of manganese atoms is kept
unchanged, consistently with the low charge transfer associated to the acid-base reactivity and
the formation of sulfite species.
In the case of the (110) and (113) surfaces, the formation of sulfate species is favored although
the formation of sulfite species appears thermodynamically possible. On the (113) surface the
formation of sulfate species is obtained only in the vicinity of the Mn4+ manganese atoms, label 2
in Figure 4f. The most stable structure is depicted in Figure 5d and the associated adsorption
energy is -4.29 eV. The electronic transfer from the SO2 molecule toward the surface involves a
large rise in the magnetic moment of the closest manganese atom from 2.77 to 4.68 μB. This can
be interpreted as the reduction Mn4+
and as a transfer of formally two electrons
from the SO2 molecule as already observed in a previous study on LiMO2 compounds 9
addition, the SO2 molecule is stabilized by the formation of secondary interaction with a free
lithium atom at the surface (interatomic distance 1.9 Å), materialized by a dashed bond in Figure
obtained by an adsorption on the last oxygen layer, label 1 in Figure 4e and is depicted in Figure
4c. The electronic transfer from the SO2 molecule toward the surface is spread over both the
oxygen atoms of the last atomic layer and one sub-surface manganese. Indeed, the electronic
structure analysis leads to a reduction of one sub-surface manganese atom from Mn4+
which is evidenced by a rise in magnetic moments from 3.31 to 3.99 μB. Simultaneously, the
electronic charges of oxygen atoms on top of which the adsorption takes place decrease form
-0.76e to -1.12e.
In conclusion, the formation of sulfate species, which involves the reduction of species on the
last atomic layers, is favored only if Mn4+
species are available on top of the surface, namely for
the (110) and (113) surfaces. On the contrary, if only Mn3+
species are available or Mn4+
buried in the sub-surface layer, the formation of sulfite species is favored which is the case for
the (111) and (001) surfaces. In addition, this conclusion can be reinforced by our previous work9
on LiMnO2 where only sulfite species were obtained when the last atomic layer contains only
cations (the (104) surface) and both sulfate and sulfite species were obtained when higher
oxidation degrees are present for manganese present at the surface (Mn4+ and Mn2+ on the (110)
The two spinel materials studied in this paper differ in their nominal Li/Mn ratio, Li1.05Mn1.95O4
and Li1.1Mn1.90O4. The slight decrease in the lattice parameter with the increasing Li/M ratio is
consistent with the increase of the Mn valence. Nonetheless, the Li/Mn ratio is different on the
surface and in the bulk of the materials, which leads to surface stoichiometries determined by
that the presence of trivalent manganese (Mn3+
) at the surface is larger than expected
The secondary electron micrographs obtained on theses samples show that only the (111),
(001) and (110) surfaces have been experimentally identified for the truncated octahedral
particles in good agreement with the spinel structure. Thus, we discuss only of those three
surfaces from a theoretical and experimental point of view.
According to the calculations on the (111), (110) and (001) surface orientations, the
manganese cations are only present in the Mn3+
oxidation state. The manganese
cations, which are located at the sub-surface layer of the (111) orientation, possesses a Mn3+/4+
mixed valence. For the other two orientations, the manganese cations at the extreme surface
exhibit a unique valence, Mn3+
for the (001) and Mn4+
for the (110) orientation. In a same
manner, the valence of the manganese has been clearly identified by XPS and in particular by
combining the information issued from the Mn 2p and Mn 3s core peaks spectra and corresponds
to a Mn3+/4+
mixed valence. As the SEM study strongly suggests a majority of (111) and (001)
surfaces, XPS results and theoretical calculations are in accordance to propose a mixed valency
of the manganese cations at the spinel surface.
After SO2 adsorption on the three considered orientations, computational results evidence the
formation of either sulfite or sulfate species. Only sulfite species are thermodynamically stable
on the (111) and (001) surfaces, whereas both sulfite and sulfate species can be obtained on the
(110) surface with a higher stability of sulfate species.
Concurrently, the adsorbed species have also been experimentally characterized by XPS after
sulfite adsorption mode for the Li1.1Mn1.90O4 spinel, while both sulfate and sulfite species were
obtained in the case of the Li1.05Mn1.95O4 spinel with sulfite species in higher quantity.
According to computational results, the sulfate species detected for the x = 0.05 spinel material
could only be linked to the redox reactivity of the (110) surfaces of the spinel crystals. Two
experimental results substantiate the assignment of the redox reactivity to the (110) surfaces: 1)
the (110) surfaces are present in a lesser amount than (111) and (110) and, 2) the acid-base
adsorption mode is predominant (69% of sulfite compared to 31% of sulfate species). In
consequence, although the amount of the different orientations was not quantified accurately, we
may suggest that the difference in the reactivity of the x = 0.1 and x = 0.05 samples is due to a
morphology change leading to a higher amount of (110) surface in the x = 0.05 sample than
x = 0.1 which can be observed from SEM imaging, Figure 2.
This argumentation, based on computational results, is strengthened by the full agreement with
the description of the electronic processes taking place, analyzed from the XPS measures.
Indeed, computational results evidence a large electronic transfer, associated to the reduction of
surface or sub-surface manganese atoms, in the case of the formation of sulfate species, while
only low transfers are obtained in the case of the formation of sulfite species, these two processes
being associated to a redox or an acid-base reactivity, respectively. Moreover, in the case of
sulfate formation on the (110) surfaces, the calculations show that the closest manganese atoms
are reduced from Mn4+
. From XPS analysis of the Mn 2p spectra decomposition after
SO2 adsorption, a noticeable increase of the Mn 3+
content (from 56 ± 1% to 60 ± 1%) has been
observed, in the case of Li1.05Mn1.95O4 material. This indicates a reduction of Mn 4+
associated to the redox adsorption process. For the Li1.1Mn1.90O4 spinel, no change in the
acid-base character of the sulfite adsorption suggested from computational and experimental
In this work, we focus on the surface reactivity of Li1+xMn2-xO4 spinel materials with two
different stoichiometries (x = 0.05 and x = 0.10). Their structure, morphology and chemical
composition were characterized in-depth. The surface reactivity was investigated through the
adsorption of a gaseous probe (SO2) in controlled conditions, and both XPS analyses and
first-principle calculations were undertaken in order to identify and quantify the adsorbed species on
the surface and characterize the surface reactivity.
The formation of both sulfite and sulfate species, associated to an acid-base and redox
reactivity, respectively, was identified from XPS analysis and computational results. Both
approaches allow us to evidence that the formation of sulfate species is only allowed in the
presence of Mn4+
cations which are reduced due to an electronic transfer from the SO2 molecule
to the surface of the material. On the contrary, only sulfite species are formed in the presence of
cations. More generally for manganese compounds, increasing the presence of manganese
atoms at the +III oxidation degree limits the redox surface reactivity.
According to the computational and experimental results, the presence of sulfate species could
be attributed to the (110) facets in the spinel crystals. In consequence, we may suggest that the
reactivity of manganese materials can be controlled by managing the shape of the crystal. Indeed,
redox reactivity could be limited in the case of spinel compounds by lowering the area of (110)
It would be worthy of continuing research and investigations in order to characterize the
proportion of each surface in the two spinel materials. Thus, we would precise the link between
the morphology and the reactivity of the spinel materials. ASSOCIATED CONTENT
Supporting Information. Mn 2p, Mn 3s, Mn 3p spectra from X-Ray Photoelectron
Spectroscopy analysis are included. Lattice parameters of calculated MnO, Mn2O3 and MnO2
materials and the manganese atoms magnetic moment are resumed. This material is available
free of charge via the Internet at http://pubs.acs.org.
CNRS/ Univ Pau & Pays Adour, Institut des Sciences Analytiques et de Physico-chimie pour
l’Environnement et les Matériaux, UMR5254, 64000, Pau, France
The authors thank the Conseil Général des Pyrénées Atlantiques and the French Research
and Christian Masquelier (LRCS-Amiens) for fruitful discussions on the spinel materials
Li1+xMn2-xO4. This project received also funding from Région Nouvelle Aquitaine and the French
National Research Agency (STORE-EX Labex Project ANR-10-LABX-76-01). The theoretical
calculations were performed using HPC resources from GENCI-CINES (Grant
2017-A0010806920) and the Mesocentre de Calcul Intensif Aquitain (MCIA).
(1) Xu, B.; Meng, S. Factors Affecting Li Mobility in Spinel LiMn2O4 - A First-Principles
Study by GGA and GGA+U Methods. J. Power Sources 2010, 195 (15), 4971–4976.
(2) Ozawa, K. Lithium-Ion Rechargeable Batteries with LiCoO2 and Carbon Electrodes: The
LiCoO2/C System. Solid State Ion. 1994, 69 (3), 212–221.
(3) Amatucci, G. G.; Pereira, N.; Zheng, T.; Tarascon, J.-M. Failure Mechanism and
Improvement of the Elevated Temperature Cycling of LiMn[Sub 2]O[Sub 4] Compounds
Through the Use of the LiAlxMn2−xO4−zFz Solid Solution. J. Electrochem. Soc. 2001, 148 (2),
(4) Amine, K.; Liu, J.; Belharouak, I.; Kang, S.-H.; Bloom, I.; Vissers, D.; Henriksen, G.
Advanced Cathode Materials for High-Power Applications. J. Power Sources 2005, 146 (1–2),
(5) Hunter, J. C. Preparation of a New Crystal Form of Manganese Dioxide: λ-MnO 2. J.
Solid State Chem. Fr. 1981, 39, 142–147.
(6) Gummow, R. J.; de Kock, A.; Thackeray, M. M. Improved Capacity Retention in
Rechargeable 4 V Lithium/Lithium-Manganese Oxide (Spinel) Cells. Solid State Ion. 1994, 69
(7) Andreu, N.; Flahaut, D.; Dedryvère, R.; Minvielle, M.; Martinez, H.; Gonbeau, D. XPS
Investigation of Surface Reactivity of Electrode Materials: Effect of the Transition Metal. ACS
Appl. Mater. Interfaces 2015, 7 (12), 6629–6636.
(8) Andreu, N.; Baraille, I.; Martinez, H.; Dedryvère, R.; Loudet, M.; Gonbeau, D. New
Investigations on the Surface Reactivity of Layered Lithium Oxides. J. Phys. Chem. C 2012, 116
(9) Vallverdu, G.; Minvielle, M.; Andreu, N.; Gonbeau, D.; Baraille, I. First Principle Study
of the Surface Reactivity of Layered Lithium Oxides LiMO2 (M = Ni, Mn, Co). Surf. Sci. 2016,
(10) Dahéron, L.; Dedryvère, R.; Martinez, H.; Flahaut, D.; Ménétrier, M.; Delmas, C.;
Gonbeau, D. Possible Explanation for the Efficiency of Al-Based Coatings on LiCoO2 : Surface
Properties of LiCo1− xAlxO2 Solid Solution. Chem. Mater. 2009, 21 (23), 5607–5616.
(11) Masquelier, C.; Tabuchi, M.; Ado, K.; Kanno, R.; Kobayashi, Y.; Maki, Y.; Nakamura,
O.; Goodenough, J. B. Chemical and Magnetic Characterization of Spinel Materials in the
LiMn2O4–Li2Mn4O9–Li4Mn5O12 System. J. Solid State Chem. 1996, 123 (2), 255–266.
(12) Bianchini, M.; Fauth, F.; Suard, E.; Leriche, J.-B.; Masquelier, C.; Croguennec, L. Spinel
Materials for Li-Ion Batteries: New Insights Obtained by Operando Neutron and Synchrotron
X-Ray Diffraction. Acta Crystallogr. Sect. B Struct. Sci. Cryst. Eng. Mater. 2015, 71 (6), 688–701.
(13) Bianchini, M.; Suard, E.; Croguennec, L.; Masquelier, C. Li-Rich Li1+xMn2–xO4 Spinel
Electrode Materials: An Operando Neutron Diffraction Study during Li+ Extraction/Insertion. J.
Phys. Chem. C 2014, 118 (45), 25947–25955.
(14) Shannon, R. D. Revised Effective Ionic Radii and Systematic Studies of Interatomic
(15) Brunauer, S.; Emmett, P. H.; Teller, E. Adsorption of Gases in Multimolecular Layers. J.
Am. Chem. Soc. 1938, 60 (2), 309–319.
(16) Lindberg, B. J.; Hamrin, K.; Johansson, G.; Gelius, U.; Fahlman, A.; Nordling, C.;
Siegbahn, K. Molecular Spectroscopy by Means of ESCA II. Sulfur Compounds. Correlation of
Electron Binding Energy with Structure. Phys. Scr. 1970, 1 (5–6), 286–298.
(17) Flahaut, D.; Minvielle, M.; Sambou, A.; Lecour, P.; Legens, C.; Barbier, J. Identification
of Sulphur, Oxygen and Nitrogen Species in Heavy Oils by X-Ray Photoelectron Spectroscopy.
Fuel 2017, 202 (Supplement C), 307–317.
(18) Guimon, C.; Gervasini, A.; Auroux, A. XPS Study of the Adsorption of SO2 and NH3
over Supported Tin Dioxide Catalysts Used in De-NOx Catalytic Reaction. J. Phys. Chem. B
2001, 105 (42), 10316–10325.
(19) Kresse, G.; Furthmüller, J. Efficient Iterative Schemes for Ab Initio Total-Energy
Calculations Using a Plane-Wave Basis Set. Phys. Rev. B 1996, 54 (16), 11169–11186.
(20) Kresse, G.; Hafner, J. Ab Initio. Phys. Rev. B 1994, 49 (20), 14251–14269.
(21) Kresse, G.; Joubert, D. From Ultrasoft Pseudopotentials to the Projector
Augmented-Wave Method. Phys. Rev. B 1999, 59 (3), 1758–1775.
(22) Perdew, J. P.; Chevary, J. A.; Vosko, S. H.; Jackson, K. A.; Pederson, M. R.; Singh, D.
J.; Fiolhais, C. Atoms, Molecules, Solids, and Surfaces: Applications of the Generalized
Gradient Approximation for Exchange and Correlation. Phys. Rev. B 1992, 46 (11), 6671–6687.
(23) Perdew, J. P.; Wang, Y. Accurate and Simple Analytic Representation of the
Electron-Gas Correlation Energy. Phys. Rev. B 1992, 45 (23), 13244–13249.
(24) Dudarev, S. L.; Botton, G. A.; Savrasov, S. Y.; Humphreys, C. J.; Sutton, A. P.
Rev. B 1998, 57 (3), 1505–1509.
(25) Henkelman, G.; Arnaldsson, A.; Jónsson, H. A Fast and Robust Algorithm for Bader
Decomposition of Charge Density. Comput. Mater. Sci. 2006, 36 (3), 354–360.
(26) Tang, W.; Sanville, E.; Henkelman, G. A Grid-Based Bader Analysis Algorithm without
Lattice Bias. J. Phys. Condens. Matter 2009, 21 (8), 084204.
(27) Kim, J.-S.; Kim, K.; Cho, W.; Shin, W. H.; Kanno, R.; Choi, J. W. A Truncated
Manganese Spinel Cathode for Excellent Power and Lifetime in Lithium-Ion Batteries. Nano
Lett. 2012, 12 (12), 6358–6365.
(28) Allen, G. C.; Harris, S. J.; Jutson, J. A.; Dyke, J. M. A Study of a Number of Mixed
Transition Metal Oxide Spinels Using X-Ray Photoelectron Spectroscopy. Appl. Surf. Sci. 1989,
37 (1), 111–134.
(29) Brabers, V. A. M.; van Setten, F. M.; Knapen, P. S. A. X-Ray Photoelectron
Spectroscopy Study of the Cation Valencies in Nickel Manganite. J. Solid State Chem. 1983, 49
(30) Berg, H.; Thomas, J. O. Neutron Diffraction Study of Electrochemically Delithiated
LiMn2O4 Spinel. Solid State Ion. 1999, 126 (3–4), 227–234.
(31) Warburton, R. E.; Iddir, H.; Curtiss, L. A.; Greeley, J. Thermodynamic Stability of Low-
and High-Index Spinel LiMn2O4 Surface Terminations. ACS Appl. Mater. Interfaces 2016, 8